# Fundamentals of cutting - PowerPoint PPT Presentation

PPT – Fundamentals of cutting PowerPoint presentation | free to download - id: 11a9c4-OTE1M

The Adobe Flash plugin is needed to view this content

Get the plugin now

View by Category
Title:

## Fundamentals of cutting

Description:

### Continuous chips are usually formed at high rake angles and/or high cutting speeds. ... ( b) View of the rake of a turning tool,showing nose radius R and crater wear ... – PowerPoint PPT presentation

Number of Views:906
Avg rating:3.0/5.0
Slides: 27
Provided by: sky22
Category:
Tags:
Transcript and Presenter's Notes

Title: Fundamentals of cutting

1
Fundamentals of cutting
• Chapter-20

2
TOPICS
• Introduction
• Mechanics of chip formation
• Types of chips produced in meta cutting
• Mechanics of oblique cutting
• Cutting forces and power
• Temperature in cutting
• Tool life Wear and failure
• Surface finish and integrity
• Machinability

3
Fundamentals of cutting
• Fig 20.3 Schematic illustration of a
two-dimensional cutting process,also called
orthogonal cutting.Note that the tool shape and
its angles,depth of cut,to,and the cutting speed
are all independent variables.

Fig 20.1 Examples of cutting process
Fig 20.2 Basic principle of turning operation
4
Introduction
• Cutting process Remove material from the
surface of the work piece by producing chips
• Turning operation the work piece is rotated an
a cutting tool removes a layer of material as it
moves to the left
• Cutting off Cutting tool moves radially inwards
and separated the right piece from the back of
the blank.
• Slab-milling rotating cutting tool removes a
layer of material from the surface of the work
piece
• End-milling rotating cutter travels along a
certain depth in the work piece and produces a
cavity

5
Factors influencing cutting process
6
Mechanics of chip formation
• Orthogonal cutting
• Rake angle Alpha
• Relief angle ( clearance angle)
• Shear angle ( Pi)
• Thickness of a chip Tc
• Depth of cut- T0
• Cutting ratio r To / Tc
• Sin Pi / Cos ( pi-
Alpha )

7
Mechanism of chip formation
• Fig 20.4 (a) Schematic illustration of the basic
mechanism of chip formation in metal cutting. (b)
Velocity diagram in the cutting zone.

8
Mechanism of chip formation
• Chip compression ratio 1 / r
• Always gt unity
• On the basis of fig 20.4-a
• Shear strain gama
• Gama AB/OC AO/OC OB/OC
• Gama Cot Pi tan ( Pi Alpha )
• Note for actual cutting operation shear strain
gt 5

9
Mechanism of chip formation
• Shear angle adjusts itself to minimize cutting
force
• Shear plane is the plane of maximum shear stress
• Pi 45 Alpha / 2 Beta / 2
• Beta Friction angle
• Mu coefficient of friction
• Mu tan beta

10
Mechanism of chip formation
• Mass continuity has to be maintained
• So , we have
• V To Vc Tc
• Vc Vr
• Vc V Sin pi / Cos ( pi Alpha )
• Vc Velocity of a chip
• V Cutting Speed
• Vs Velocity of shearing
• From trigonometric relation
• V / cos ( pi Alpha ) Vs / Cos ( Alpha ) Vc
/ Sin ( pi )

11
Types of chips
• Continuous
• Built up edge
• Serrated or segmented
• Discontinuous
• Fig20.5 Basic types of chips and their
photomicrographs produced in metal cutting (a)
continuous ship with a narrow,straight primary
shear zone (b) secondary shear zone at the chip
tool interface(c) continuous chip with large
primary shear zone (d) continuous chip with
built-up-edge(e) segmented or nonhomogeneous
chip and (f) discontinuous chips

12
Continuous chips
(b) Surface finish in turning 5130 steel with a
built-up edge
• Fig 20.6 (a) Hardness distribution in the
cutting zone for 3115 steel.Note that some
regions in the built-up edge are as mach as three
times harder than the bulk metal

(c) Surface finish on 1018 steel in face milling
13
Continuous chips
• Continuous chips are usually formed at high rake
angles and/or high cutting speeds.
• A good surface finish is generally produced.
• continuous chips are not always desirable,
particularly in automated machine tools,
• tend to get tangled around the tool
• operation has to be stopped to clear away the
chips.

14
Built-up edges chips
• BUE consists of layers of material from the
workpiece that are gradually deposited on the
tool.
• BUE then becomes unstable and eventually breaks
up
• BUE material is carried away on the tool side of
the chip
• the rest is deposited randomly on the workpiece
surface.
• BUE results in poor surface finish
• reduced by increasing the rake angle and
therefore decreasing the depth of cut.

15
Discontinuous chips
• Discontinuous chips consist of segments that may
be firmly or loosely attached to each other
• These chips occur when machining hard brittle
materials such as cast iron.
• Brittle failure takes place along the shear plane
before any tangible plastic flow occurs
• Discontinuous chips will form in brittle
materials at low rake angles (large depths of
cut).

16
Serrated chips
• Figure 20.5e
• Segmented chips or non-homogeneous chips
• Semi continuous chips with zones low and high
shear strain
• Low thermal conductivity and strength metals
exhibit this behavior

Fig 20.5 (e)segmented or nonhomogeneous chip and
17
Chip Breakers
• Long continuous chip are undesirable
• Chip breaker is a piece of metal clamped to the
rake surface of the tool which bends the chip and
breaks it
• Chips can also be broken by changing the tool
geometry,thereby controlling the chip flow
• Fig 20.7 (a) Schematic illustration of the action
of a chip breaker .(b) Chip breaker clamped on
the rake of a cutting tool. (c) Grooves in
cutting tools acting as chip breakers

18
Chip Breakers
FigVarious chips produced in turning a)tightly
curled chip b)chip hits workpiece and breaks
c)continuous chip moving away from workpieceand
d)chip hits tool shank and breaks off
19
Chip Formation in Nonmetallic Materials
Fig a) cutting with an oblique tool b) Top view
showing the inclination angle, i. c) Types of
chips produced with different inclination
20
Mechanism of Oblique Cutting
• The cutting edge is at an angle i, called
inclination angle.
• The chip movement is in lateral direction
• Fig a)right hand cutting tool.Although these
tools have traditionally been produced from
solids tool-steel bars,they have been largely
replaced by carbide or other inserts of various
shapes and sizes,as shownin b).The vcarious
angles on these tools and their effects on
machining are described

21
Temperature In Cutting
FigPercentage of the heat generated in cutting
going into the workpiece,tool,and chip,as a
function of cutting speed.
FigTypical temperature distribution in the
cutting zone.
22
Temperature Distributions
FigTemperatures developed in turning 52100
steel a) flank temperature distributionand
b)tool-chip interface temperature distribution
23
Tool Life Wear and Failure
• Flank wear It occurs on the relief face of the
tool and the side relief angle.
• Crater wearIt occurs on the rake face of the
tool.
• Chipping Breaking away of a small piece from the
cutting edge of the tool .
• Fig (a) Flank and crater wear in a cutting
tool.tool moves to the left. (b) View of the rake
of a turning tool,showing nose radius R and
crater wear pattern on the rake face of the tool
c)View of the flank face of a turning tool,sowing
the average flank wear land VB and the
depth-of-cut line (wear notch)

24
Wear and Tool Failures Crater wear
• Fig (a) Schematic illustrations of types of wear
observed on various types of cutting tools .(b)
Schematic illustrations of catastrophic tool
failures.A study of the types and mechanism of
tool wear and failure is essential to the
development of better tool materials

25
Forces acting in 2-Dimensional cutting
• Cutting forces can be measured by using suitable
dynamometers or force transducers mounted on the
machine tool
• They can also be calculated from the amount of
power consumption,that occurs during cutting.
• Fig Forces acting on a cutting tool in a two
dimensional cutting .Note that the resultant
force,R,must be collinear to balance the forces

26
THE END